#------------------------------------------------------------------------------
#$Date: 2021-07-16 08:10:18 +0300 (Fri, 16 Jul 2021) $
#$Revision: 267586 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/88/2108838.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2108838
loop_
_publ_author_name
'Ballirano, Paolo'
'Celata, Beatrice'
'Pacella, Alessandro'
'Bosi, Ferdinando'
_publ_section_title
;
 Recommended X-ray single-crystal structure refinement and Rietveld
 refinement procedure for tremolite
;
_journal_coeditor_code           YH5012SUP1
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first
;
;
_journal_paper_doi               10.1107/S2052520621004844
_journal_volume                  77
_journal_year                    2021
_chemical_formula_moiety
'F0.33 Mg5.09 O13.67, 0.05(K4), 7.32(Si), 10(O), 1.99(Ca), 0.68(Al), 1.61(H)'
_chemical_formula_sum
'Al0.68 Ca1.99 F0.33 H1.61 K0.2 Mg5.09 O23.67 Si7.32'
_chemical_formula_weight         821.80
_chemical_name_common            tremolite
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_atom_sites_solution_hydrogens   difmap
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2021-02-19 # Formatted by publCIF

;
_cell_angle_alpha                90
_cell_angle_beta                 104.9961(8)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.8348(3)
_cell_length_b                   18.0035(6)
_cell_length_c                   5.2825(2)
_cell_measurement_reflns_used    9978
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      40.3
_cell_measurement_theta_min      4
_cell_volume                     903.47(5)
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 512
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker KAPPA APEX-II'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0171
_diffrn_reflns_av_unetI/netI     0.0095
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            20233
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         40.302
_diffrn_reflns_theta_min         3.994
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    1.512
_exptl_absorpt_correction_T_max  0.7479
_exptl_absorpt_correction_T_min  0.6670
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Bruker, 2003)'
_exptl_crystal_colour            pale-green
_exptl_crystal_density_diffrn    3.021
_exptl_crystal_description       gem-quality
_exptl_crystal_F_000             868
_exptl_crystal_size_max          0.310
_exptl_crystal_size_mid          0.220
_exptl_crystal_size_min          0.210
_exptl_transmission_factor_max   0.712
_exptl_transmission_factor_min   0.659
_refine_diff_density_max         0.644
_refine_diff_density_min         -0.316
_refine_diff_density_rms         0.058
_refine_ls_extinction_coef       0.0204(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick, 2018)'
_refine_ls_goodness_of_fit_ref   1.117
_refine_ls_hydrogen_treatment    refxyz
_refine_ls_matrix_type           full
_refine_ls_number_parameters     111
_refine_ls_number_reflns         2920
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.117
_refine_ls_R_factor_all          0.0147
_refine_ls_R_factor_gt           0.0132
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0119P)²+0.3014P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0309
_refine_ls_wR_factor_ref         0.0314
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2763
_reflns_number_total             2920
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            yh5012sup1.cif
_cod_data_source_block           tremolite
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_original_formula_sum
'Al0.68 Ca1.99 F0.33 H1.61 K0.20 Mg5.09 O23.67 Si7.32'
_cod_database_code               2108838
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.634
_shelx_estimated_absorpt_t_max   0.727
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
M1 Mg 0.000000 0.08833(2) 0.500000 0.00580(6) Uani 1.0104(16) 2 d S T . . .
M2 Mg 0.000000 0.17645(2) 0.000000 0.00470(5) Uani 1.0309(15) 2 d S T . . .
M3 Mg 0.000000 0.000000 0.000000 0.00537(8) Uani 1.005(2) 4 d S T . . .
M4 Ca 0.000000 0.27880(2) 0.500000 0.00858(3) Uani 0.9939(10) 2 d S T . . .
T1 Si 0.28019(2) 0.08467(2) 0.29965(2) 0.00451(3) Uani 0.646(11) 1 d . . P . .
T1A Si 0.28019(2) 0.08467(2) 0.29965(2) 0.00451(3) Uani 0.184(11) 1 d . . P . .
T1AL Al 0.28019(2) 0.08467(2) 0.29965(2) 0.00451(3) Uani 0.17 1 d . . P . .
T2 Si 0.28906(2) 0.17207(2) 0.80829(2) 0.00486(3) Uani 0.778(13) 1 d . . P . .
T2A Si 0.28906(2) 0.17207(2) 0.80829(2) 0.00486(3) Uani 0.222(13) 1 d . . P . .
O1 O 0.10950(3) 0.08663(2) 0.21737(6) 0.00698(5) Uani 0.356(13) 1 d . . P . .
O1A O 0.10950(3) 0.08663(2) 0.21737(6) 0.00698(5) Uani 0.644(13) 1 d . . P . .
O2 O 0.11848(3) 0.17170(2) 0.72769(6) 0.00662(5) Uani 0.356(13) 1 d . . P . .
O2A O 0.11848(3) 0.17170(2) 0.72769(6) 0.00662(5) Uani 0.644(13) 1 d . . P . .
O3 O 0.10874(5) 0.000000 0.71547(9) 0.00803(7) Uani 0.297(11) 2 d S T P . .
O3A O 0.10874(5) 0.000000 0.71547(9) 0.00803(7) Uani 0.538(11) 2 d S T P . .
H H 0.2088(15) 0.000000 0.773(3) 0.010 Uiso 0.8045 2 d S U P . .
F3 F 0.10874(5) 0.000000 0.71547(9) 0.00803(7) Uani 0.1655 2 d S T P . .
O4 O 0.36560(3) 0.24926(2) 0.79264(7) 0.00875(5) Uani 0.356(13) 1 d . . P . .
O4A O 0.36560(3) 0.24926(2) 0.79264(7) 0.00875(5) Uani 0.644(13) 1 d . . P . .
O5 O 0.34758(3) 0.13648(2) 0.10495(6) 0.00936(6) Uani 0.356(13) 1 d . . P . .
O5A O 0.34758(3) 0.13648(2) 0.10495(6) 0.00936(6) Uani 0.644(13) 1 d . . P . .
O6 O 0.34375(3) 0.11849(2) 0.59634(6) 0.00867(5) Uani 0.356(13) 1 d . . P . .
O6A O 0.34375(3) 0.11849(2) 0.59634(6) 0.00867(5) Uani 0.644(13) 1 d . . P . .
O7 O 0.33729(5) 0.000000 0.29008(10) 0.01064(8) Uani 0.356(13) 2 d S T P . .
O7A O 0.33729(5) 0.000000 0.29008(10) 0.01064(8) Uani 0.644(13) 2 d S T P . .
AM K 0.0271(5) 0.500000 0.0571(9) 0.0516(16) Uani 0.1004(13) 2 d S T . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O 'O 1-' 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O 'O neutral' 0.0106 0.0060
'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O 'O 2-' 0.0106 0.0060 'Hovestreydt, 1983'
Si 'Si 4+' 0.0720 0.0710
'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 M1 O1 178.29(2) . 2_556 ?
O1 M1 O2 96.335(13) . . ?
O1 M1 O2 84.904(13) 2_556 . ?
O1 M1 O2 84.903(13) . 2_556 ?
O1 M1 O2 96.334(13) 2_556 2_556 ?
O2 M1 O2 87.706(19) . 2_556 ?
O1 M1 O3 95.404(16) . . ?
O1 M1 O3 83.284(16) 2_556 . ?
O2 M1 O3 95.927(13) . . ?
O2 M1 O3 176.292(15) 2_556 . ?
O1 M1 O3 83.284(16) . 5_556 ?
O1 M1 O3 95.404(16) 2_556 5_556 ?
O2 M1 O3 176.293(15) . 5_556 ?
O2 M1 O3 95.927(13) 2_556 5_556 ?
O3 M1 O3 80.45(2) . 5_556 ?
O1 M1 M2 42.988(10) . . ?
O1 M1 M2 138.317(11) 2_556 . ?
O2 M1 M2 89.995(11) . . ?
O2 M1 M2 42.054(9) 2_556 . ?
O3 M1 M2 138.392(13) . . ?
O3 M1 M2 92.209(11) 5_556 . ?
O1 M1 M2 138.317(11) . 1_556 ?
O1 M1 M2 42.989(10) 2_556 1_556 ?
O2 M1 M2 42.053(9) . 1_556 ?
O2 M1 M2 89.994(11) 2_556 1_556 ?
O3 M1 M2 92.210(11) . 1_556 ?
O3 M1 M2 138.392(13) 5_556 1_556 ?
M2 M1 M2 118.019(10) . 1_556 ?
O4 M2 O4 95.89(2) 7_556 8_454 ?
O4 M2 O2 89.836(13) 7_556 1_554 ?
O4 M2 O2 93.331(13) 8_454 1_554 ?
O4 M2 O2 93.331(13) 7_556 2_556 ?
O4 M2 O2 89.836(13) 8_454 2_556 ?
O2 M2 O2 175.27(2) 1_554 2_556 ?
O4 M2 O1 92.441(13) 7_556 . ?
O4 M2 O1 169.740(14) 8_454 . ?
O2 M2 O1 92.672(13) 1_554 . ?
O2 M2 O1 83.695(13) 2_556 . ?
O4 M2 O1 169.741(14) 7_556 2 ?
O4 M2 O1 92.441(13) 8_454 2 ?
O2 M2 O1 83.696(13) 1_554 2 ?
O2 M2 O1 92.672(13) 2_556 2 ?
O1 M2 O1 79.958(18) . 2 ?
O4 M2 M1 91.228(10) 7_556 . ?
O4 M2 M1 131.942(10) 8_454 . ?
O2 M2 M1 134.262(11) 1_554 . ?
O2 M2 M1 42.234(9) 2_556 . ?
O1 M2 M1 41.597(9) . . ?
O1 M2 M1 87.635(11) 2 . ?
O4 M2 M1 131.942(10) 7_556 1_554 ?
O4 M2 M1 91.229(10) 8_454 1_554 ?
O2 M2 M1 42.235(9) 1_554 1_554 ?
O2 M2 M1 134.261(11) 2_556 1_554 ?
O1 M2 M1 87.634(11) . 1_554 ?
O1 M2 M1 41.597(9) 2 1_554 ?
M1 M2 M1 118.019(10) . 1_554 ?
O4 M2 M3 132.056(11) 7_556 . ?
O4 M2 M3 132.056(11) 8_454 . ?
O2 M2 M3 87.637(10) 1_554 . ?
O2 M2 M3 87.637(10) 2_556 . ?
O1 M2 M3 39.979(9) . . ?
O1 M2 M3 39.979(9) 2 . ?
M1 M2 M3 59.010(5) . . ?
M1 M2 M3 59.010(5) 1_554 . ?
O4 M2 M4 85.769(11) 7_556 1_554 ?
O4 M2 M4 46.154(10) 8_454 1_554 ?
O2 M2 M4 48.360(9) 1_554 1_554 ?
O2 M2 M4 135.368(11) 2_556 1_554 ?
O1 M2 M4 140.933(9) . 1_554 ?
O1 M2 M4 95.764(9) 2 1_554 ?
M1 M2 M4 176.090(7) . 1_554 ?
M1 M2 M4 65.890(5) 1_554 1_554 ?
M3 M2 M4 124.900(4) . 1_554 ?
O4 M2 M4 46.153(10) 7_556 . ?
O4 M2 M4 85.768(12) 8_454 . ?
O2 M2 M4 135.368(11) 1_554 . ?
O2 M2 M4 48.360(9) 2_556 . ?
O1 M2 M4 95.765(9) . . ?
O1 M2 M4 140.934(9) 2 . ?
M1 M2 M4 65.891(5) . . ?
M1 M2 M4 176.090(7) 1_554 . ?
M3 M2 M4 124.901(4) . . ?
M4 M2 M4 110.200(8) 1_554 . ?
O3 M3 O3 180.000(18) 5_556 1_554 ?
O3 M3 O1 83.612(12) 5_556 . ?
O3 M3 O1 96.388(12) 1_554 . ?
O3 M3 O1 96.388(12) 5_556 5 ?
O3 M3 O1 83.612(12) 1_554 5 ?
O1 M3 O1 180.000(16) . 5 ?
O3 M3 O1 83.612(12) 5_556 6 ?
O3 M3 O1 96.388(12) 1_554 6 ?
O1 M3 O1 97.999(18) . 6 ?
O1 M3 O1 82.001(18) 5 6 ?
O3 M3 O1 96.388(12) 5_556 2 ?
O3 M3 O1 83.612(12) 1_554 2 ?
O1 M3 O1 82.001(18) . 2 ?
O1 M3 O1 97.999(18) 5 2 ?
O1 M3 O1 180.000(12) 6 2 ?
O3 M3 M1 137.810(8) 5_556 5 ?
O3 M3 M1 42.190(8) 1_554 5 ?
O1 M3 M1 138.573(9) . 5 ?
O1 M3 M1 41.428(9) 5 5 ?
O1 M3 M1 88.350(10) 6 5 ?
O1 M3 M1 91.650(10) 2 5 ?
O3 M3 M1 42.190(8) 5_556 5_556 ?
O3 M3 M1 137.810(8) 1_554 5_556 ?
O1 M3 M1 91.650(10) . 5_556 ?
O1 M3 M1 88.351(10) 5 5_556 ?
O1 M3 M1 41.428(9) 6 5_556 ?
O1 M3 M1 138.572(9) 2 5_556 ?
M1 M3 M1 117.896(8) 5 5_556 ?
O3 M3 M1 137.810(8) 5_556 1_554 ?
O3 M3 M1 42.190(8) 1_554 1_554 ?
O1 M3 M1 88.350(10) . 1_554 ?
O1 M3 M1 91.649(10) 5 1_554 ?
O1 M3 M1 138.572(9) 6 1_554 ?
O1 M3 M1 41.428(9) 2 1_554 ?
M1 M3 M1 62.104(8) 5 1_554 ?
M1 M3 M1 180.0 5_556 1_554 ?
O3 M3 M1 42.190(8) 5_556 . ?
O3 M3 M1 137.810(8) 1_554 . ?
O1 M3 M1 41.427(9) . . ?
O1 M3 M1 138.573(9) 5 . ?
O1 M3 M1 91.650(10) 6 . ?
O1 M3 M1 88.350(10) 2 . ?
M1 M3 M1 180.0 5 . ?
M1 M3 M1 62.105(7) 5_556 . ?
M1 M3 M1 117.895(7) 1_554 . ?
O3 M3 M2 90.0 5_556 . ?
O3 M3 M2 90.0 1_554 . ?
O1 M3 M2 41.000(9) . . ?
O1 M3 M2 138.999(9) 5 . ?
O1 M3 M2 138.999(9) 6 . ?
O1 M3 M2 41.001(9) 2 . ?
M1 M3 M2 121.052(4) 5 . ?
M1 M3 M2 121.052(4) 5_556 . ?
M1 M3 M2 58.948(4) 1_554 . ?
M1 M3 M2 58.948(4) . . ?
O4 M4 O4 155.006(17) 8_455 7_556 ?
O4 M4 O2 82.746(12) 8_455 2_556 ?
O4 M4 O2 77.272(11) 7_556 2_556 ?
O4 M4 O2 77.272(11) 8_455 . ?
O4 M4 O2 82.747(12) 7_556 . ?
O2 M4 O2 73.581(15) 2_556 . ?
O4 M4 O6 140.016(12) 8_455 7_556 ?
O4 M4 O6 63.194(11) 7_556 7_556 ?
O2 M4 O6 136.304(11) 2_556 7_556 ?
O2 M4 O6 116.338(11) . 7_556 ?
O4 M4 O6 63.194(11) 8_455 8_455 ?
O4 M4 O6 140.016(12) 7_556 8_455 ?
O2 M4 O6 116.337(11) 2_556 8_455 ?
O2 M4 O6 136.304(11) . 8_455 ?
O6 M4 O6 86.492(15) 7_556 8_455 ?
O4 M4 O5 84.653(11) 8_455 7_556 ?
O4 M4 O5 109.716(11) 7_556 7_556 ?
O2 M4 O5 159.621(11) 2_556 7_556 ?
O2 M4 O5 88.065(11) . 7_556 ?
O6 M4 O5 60.019(10) 7_556 7_556 ?
O6 M4 O5 71.203(11) 8_455 7_556 ?
O4 M4 O5 109.716(11) 8_455 8_455 ?
O4 M4 O5 84.653(11) 7_556 8_455 ?
O2 M4 O5 88.065(11) 2_556 8_455 ?
O2 M4 O5 159.621(11) . 8_455 ?
O6 M4 O5 71.203(11) 7_556 8_455 ?
O6 M4 O5 60.019(10) 8_455 8_455 ?
O5 M4 O5 111.308(15) 7_556 8_455 ?
O4 M4 T2 170.587(9) 8_455 7_556 ?
O4 M4 T2 30.429(9) 7_556 7_556 ?
O2 M4 T2 105.722(8) 2_556 7_556 ?
O2 M4 T2 100.894(8) . 7_556 ?
O6 M4 T2 32.791(8) 7_556 7_556 ?
O6 M4 T2 114.979(9) 8_455 7_556 ?
O5 M4 T2 86.062(8) 7_556 7_556 ?
O5 M4 T2 75.205(8) 8_455 7_556 ?
O4 M4 T2 30.429(9) 8_455 8_455 ?
O4 M4 T2 170.587(9) 7_556 8_455 ?
O2 M4 T2 100.893(8) 2_556 8_455 ?
O2 M4 T2 105.722(8) . 8_455 ?
O6 M4 T2 114.979(9) 7_556 8_455 ?
O6 M4 T2 32.791(8) 8_455 8_455 ?
O5 M4 T2 75.205(8) 7_556 8_455 ?
O5 M4 T2 86.062(8) 8_455 8_455 ?
T2 M4 T2 146.622(7) 7_556 8_455 ?
O4 M4 M2 38.087(8) 8_455 1_556 ?
O4 M4 M2 122.647(10) 7_556 1_556 ?
O2 M4 M2 81.305(9) 2_556 1_556 ?
O2 M4 M2 40.075(8) . 1_556 ?
O6 M4 M2 135.205(8) 7_556 1_556 ?
O6 M4 M2 97.116(8) 8_455 1_556 ?
O5 M4 M2 78.897(8) 7_556 1_556 ?
O5 M4 M2 146.948(7) 8_455 1_556 ?
T2 M4 M2 137.807(3) 7_556 1_556 ?
T2 M4 M2 65.652(4) 8_455 1_556 ?
O1 T1 O7 110.68(2) . . ?
O1 T1 O6 111.018(17) . . ?
O7 T1 O6 109.06(2) . . ?
O1 T1 O5 112.065(17) . . ?
O7 T1 O5 108.20(2) . . ?
O6 T1 O5 105.642(18) . . ?
O1 T1 M3 34.484(12) . . ?
O7 T1 M3 78.341(17) . . ?
O6 T1 M3 135.714(13) . . ?
O5 T1 M3 113.325(13) . . ?
O1 T1 M1 33.644(12) . . ?
O7 T1 M1 111.278(18) . . ?
O6 T1 M1 79.906(12) . . ?
O5 T1 M1 135.599(13) . . ?
M3 T1 M1 57.731(4) . . ?
O1 T1 M2 33.946(12) . . ?
O7 T1 M2 135.694(18) . . ?
O6 T1 M2 109.914(13) . . ?
O5 T1 M2 80.543(12) . . ?
M3 T1 M2 59.104(4) . . ?
M1 T1 M2 57.066(4) . . ?
O1 T1 M4 128.554(13) . 7_556 ?
O7 T1 M4 120.656(17) . 7_556 ?
O6 T1 M4 49.932(12) . 7_556 ?
O5 T1 M4 55.731(13) . 7_556 ?
M3 T1 M4 159.381(4) . 7_556 ?
M1 T1 M4 115.614(5) . 7_556 ?
M2 T1 M4 100.481(5) . 7_556 ?
O4 T2 O2 117.453(18) . . ?
O4 T2 O5 109.530(19) . 1_556 ?
O2 T2 O5 109.290(17) . 1_556 ?
O4 T2 O6 103.347(18) . . ?
O2 T2 O6 108.225(17) . . ?
O5 T2 O6 108.568(18) 1_556 . ?
O4 T2 M4 47.930(13) . 7_556 ?
O2 T2 M4 130.950(13) . 7_556 ?
O5 T2 M4 119.725(13) 1_556 7_556 ?
O6 T2 M4 55.473(13) . 7_556 ?
O4 T2 M2 117.218(14) . 1_556 ?
O2 T2 M2 32.227(12) . 1_556 ?
O5 T2 M2 80.346(12) 1_556 1_556 ?
O6 T2 M2 132.960(13) . 1_556 ?
M4 T2 M2 156.802(5) 7_556 1_556 ?
O4 T2 M1 137.808(14) . . ?
O2 T2 M1 32.487(12) . . ?
O5 T2 M1 109.835(13) 1_556 . ?
O6 T2 M1 77.767(12) . . ?
M4 T2 M1 119.253(5) 7_556 . ?
M2 T2 M1 56.459(3) 1_556 . ?
O4 T2 M4 80.401(13) . . ?
O2 T2 M4 37.993(12) . . ?
O5 T2 M4 134.595(13) 1_556 . ?
O6 T2 M4 111.869(13) . . ?
M4 T2 M4 100.080(4) 7_556 . ?
M2 T2 M4 57.122(3) 1_556 . ?
M1 T2 M4 61.209(5) . . ?
O4 T2 AM 123.12(6) . 7_556 ?
O2 T2 AM 119.08(6) . 7_556 ?
O5 T2 AM 55.92(7) 1_556 7_556 ?
O6 T2 AM 52.88(8) . 7_556 ?
M4 T2 AM 88.78(7) 7_556 7_556 ?
M2 T2 AM 113.43(7) 1_556 7_556 ?
M1 T2 AM 91.70(6) . 7_556 ?
M4 T2 AM 152.49(6) . 7_556 ?
T1 O1 M1 120.420(18) . . ?
T1 O1 M3 119.132(18) . . ?
M1 O1 M3 96.850(14) . . ?
T1 O1 M2 120.636(18) . . ?
M1 O1 M2 95.415(14) . . ?
M3 O1 M2 99.021(14) . . ?
T2 O2 M2 123.148(18) . 1_556 ?
T2 O2 M1 122.791(18) . . ?
M2 O2 M1 95.714(13) 1_556 . ?
T2 O2 M4 117.530(17) . . ?
M2 O2 M4 91.563(13) 1_556 . ?
M1 O2 M4 99.357(13) . . ?
M3 O3 M1 96.244(15) 1_556 5_556 ?
M3 O3 M1 96.244(15) 1_556 . ?
M1 O3 M1 99.55(2) 5_556 . ?
M3 O3 H 117.2(9) 1_556 . ?
M1 O3 H 121.1(4) 5_556 . ?
M1 O3 H 121.1(4) . . ?
T2 O4 M2 144.16(2) . 7_556 ?
T2 O4 M4 101.641(17) . 7_556 ?
M2 O4 M4 95.758(13) 7_556 7_556 ?
T1 O5 T2 135.49(2) . 1_554 ?
T1 O5 M4 94.000(15) . 7_556 ?
T2 O5 M4 120.040(18) 1_554 7_556 ?
T1 O5 AM 88.61(8) . 7 ?
T2 O5 AM 96.67(8) 1_554 7 ?
M4 O5 AM 120.01(8) 7_556 7 ?
T1 O5 AM 86.05(8) . 3_545 ?
T2 O5 AM 107.37(8) 1_554 3_545 ?
M4 O5 AM 107.40(7) 7_556 3_545 ?
AM O5 AM 13.03(16) 7 3_545 ?
T1 O6 T2 138.04(2) . . ?
T1 O6 M4 100.311(16) . 7_556 ?
T2 O6 M4 91.737(15) . 7_556 ?
T1 O6 AM 109.09(7) . 7_556 ?
T2 O6 AM 99.63(9) . 7_556 ?
M4 O6 AM 118.43(8) 7_556 7_556 ?
T1 O6 AM 116.86(5) . 3_546 ?
T2 O6 AM 94.94(7) . 3_546 ?
M4 O6 AM 111.46(6) 7_556 3_546 ?
AM O6 AM 8.80(11) 7_556 3_546 ?
T1 O7 T1 138.55(3) . 6 ?
T1 O7 AM 108.91(2) . 3_545 ?
T1 O7 AM 108.91(2) 6 3_545 ?
T1 O7 AM 105.83(3) . 7 ?
T1 O7 AM 105.83(3) 6 7 ?
AM O7 AM 15.85(19) 3_545 7 ?
T1 O7 AM 90.95(3) . 7_556 ?
T1 O7 AM 90.95(3) 6 7_556 ?
AM O7 AM 111.00(11) 3_545 7_556 ?
AM O7 AM 126.85(15) 7 7_556 ?
AM AM O7 85.7(8) 5_565 3_455 ?
AM AM O7 78.4(8) 5_565 7 ?
O7 AM O7 164.15(19) 3_455 7 ?
AM AM O6 131.70(13) 5_565 4_556 ?
O7 AM O6 87.11(12) 3_455 4_556 ?
O7 AM O6 103.40(12) 7 4_556 ?
AM AM O6 131.70(13) 5_565 7_556 ?
O7 AM O6 87.11(12) 3_455 7_556 ?
O7 AM O6 103.40(12) 7 7_556 ?
O6 AM O6 95.44(12) 4_556 7_556 ?
AM AM O5 91.8(5) 5_565 4 ?
O7 AM O5 124.25(8) 3_455 4 ?
O7 AM O5 57.03(8) 7 4 ?
O6 AM O5 54.82(4) 4_556 4 ?
O6 AM O5 130.31(15) 7_556 4 ?
AM AM O5 91.8(5) 5_565 7 ?
O7 AM O5 124.25(8) 3_455 7 ?
O7 AM O5 57.03(8) 7 7 ?
O6 AM O5 130.31(15) 4_556 7 ?
O6 AM O5 54.82(4) 7_556 7 ?
O5 AM O5 111.50(15) 4 7 ?
AM AM O5 75.2(4) 5_565 8_455 ?
O7 AM O5 55.87(7) 3_455 8_455 ?
O7 AM O5 118.75(10) 7 8_455 ?
O6 AM O5 135.02(17) 4_556 8_455 ?
O6 AM O5 61.60(4) 7_556 8_455 ?
O5 AM O5 166.97(16) 4 8_455 ?
O5 AM O5 69.681(18) 7 8_455 ?
AM AM O5 75.2(4) 5_565 3_455 ?
O7 AM O5 55.87(7) 3_455 3_455 ?
O7 AM O5 118.75(10) 7 3_455 ?
O6 AM O5 61.60(4) 4_556 3_455 ?
O6 AM O5 135.02(17) 7_556 3_455 ?
O5 AM O5 69.681(18) 4 3_455 ?
O5 AM O5 166.97(16) 7 3_455 ?
O5 AM O5 106.14(14) 8_455 3_455 ?
AM AM O7 154.7(9) 5_565 7_556 ?
O7 AM O7 69.00(11) 3_455 7_556 ?
O7 AM O7 126.85(15) 7 7_556 ?
O6 AM O7 49.88(7) 4_556 7_556 ?
O6 AM O7 49.88(7) 7_556 7_556 ?
O5 AM O7 102.20(9) 4 7_556 ?
O5 AM O7 102.20(9) 7 7_556 ?
O5 AM O7 89.97(10) 8_455 7_556 ?
O5 AM O7 89.97(10) 3_455 7_556 ?
AM AM T1 86.0(7) 5_565 7 ?
O7 AM T1 151.75(6) 3_455 7 ?
O7 AM T1 27.78(4) 7 7 ?
O6 AM T1 118.12(14) 4_556 7 ?
O6 AM T1 78.51(7) 7_556 7 ?
O5 AM T1 82.96(11) 4 7 ?
O5 AM T1 29.34(4) 7 7 ?
O5 AM T1 95.89(5) 8_455 7 ?
O5 AM T1 145.80(13) 3_455 7 ?
O7 AM T1 116.31(11) 7_556 7 ?
AM AM T1 86.0(7) 5_565 4 ?
O7 AM T1 151.75(6) 3_455 4 ?
O7 AM T1 27.78(4) 7 4 ?
O6 AM T1 78.51(7) 4_556 4 ?
O6 AM T1 118.12(14) 7_556 4 ?
O5 AM T1 29.34(4) 4 4 ?
O5 AM T1 82.96(11) 7 4 ?
O5 AM T1 145.80(13) 8_455 4 ?
O5 AM T1 95.89(5) 3_455 4 ?
O7 AM T1 116.31(11) 7_556 4 ?
T1 AM T1 53.89(7) 7 4 ?
AM AM H 143.0(9) 5_565 7_556 ?
O7 AM H 131.3(4) 3_455 7_556 ?
O7 AM H 64.6(3) 7 7_556 ?
O6 AM H 61.9(2) 4_556 7_556 ?
O6 AM H 61.9(2) 7_556 7_556 ?
O5 AM H 68.69(18) 4 7_556 ?
O5 AM H 68.69(18) 7 7_556 ?
O5 AM H 122.12(13) 8_455 7_556 ?
O5 AM H 122.12(13) 3_455 7_556 ?
O7 AM H 62.3(3) 7_556 7_556 ?
T1 AM H 61.4(3) 7 7_556 ?
T1 AM H 61.4(3) 4 7_556 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
M1 O1 2.0546(3) . ?
M1 O1 2.0546(3) 2_556 ?
M1 O2 2.0813(4) . ?
M1 O2 2.0813(4) 2_556 ?
M1 O3 2.0829(3) . ?
M1 O3 2.0829(3) 5_556 ?
M1 M2 3.08105(18) . ?
M1 M2 3.08108(18) 1_556 ?
M2 O4 1.9967(4) 7_556 ?
M2 O4 1.9967(4) 8_454 ?
M2 O2 2.0741(3) 1_554 ?
M2 O2 2.0741(3) 2_556 ?
M2 O1 2.1102(4) . ?
M2 O1 2.1102(4) 2 ?
M2 M3 3.1767(2) . ?
M2 M4 3.22043(16) 1_554 ?
M2 M4 3.22047(16) . ?
M3 O3 2.0578(5) 5_556 ?
M3 O3 2.0578(5) 1_554 ?
M3 O1 2.0666(3) . ?
M3 O1 2.0666(3) 5 ?
M3 O1 2.0666(3) 6 ?
M3 O1 2.0666(3) 2 ?
M4 O4 2.3344(3) 8_455 ?
M4 O4 2.3344(3) 7_556 ?
M4 O2 2.4077(3) 2_556 ?
M4 O2 2.4077(3) . ?
M4 O6 2.5386(4) 7_556 ?
M4 O6 2.5386(4) 8_455 ?
M4 O5 2.7037(4) 7_556 ?
M4 O5 2.7037(4) 8_455 ?
M4 T2 3.08001(14) 7_556 ?
M4 T2 3.08001(14) 8_455 ?
T1 O1 1.6220(3) . ?
T1 O7 1.6298(2) . ?
T1 O6 1.6464(3) . ?
T1 O5 1.6492(3) . ?
T2 O4 1.5927(3) . ?
T2 O2 1.6205(3) . ?
T2 O5 1.6526(3) 1_556 ?
T2 O6 1.6688(3) . ?
T2 AM 3.565(2) 7_556 ?
O3 H 0.952(14) . ?
O5 AM 2.973(3) 7 ?
O5 AM 3.074(3) 3_545 ?
O6 AM 2.883(3) 7_556 ?
O6 AM 3.384(3) 3_546 ?
O7 AM 2.487(5) 3_545 ?
O7 AM 2.532(5) 7 ?
O7 AM 3.360(4) 7_556 ?
AM AM 0.693(8) 5_565 ?

_cod_database_fobs_code 2108838
